Journal of Non-Crystalline Solids 266±269 (2000) 765±768 www.elsevier.com/locate/jnoncrysol Determination of bonding in amorphous carbons by electron energy loss spectroscopy, Raman scattering and X-ray re¯ectivity A.C. Ferrari a, B. Kleinsorge a, G. Adamopoulos a, J. Robertson a,*, W.I. Milne a, V. Stolojan b, L.M. Brown b, A. LiBassi c, B.K. Tanner c a Department of Engineering, Cambridge University, Trumpington Street, Cambridge CB2 1PZ, UK b Cavendish Labs, Cambridge University, Cambridge CB3 0HE, UK c Department of Physics, Durham University, Durham, UK Abstract X-ray re¯ectivity (XRR) and Raman scattering are developed as non-destructive methods to ®nd the density and sp3 content of unhydrogenated and hydrogenated amorphous carbon ®lms. An empirical relationship is found to derive the sp3 fraction from visible Raman spectra, while ultraviolet (UV) Raman is able to directly detect sp3 sites. The sp3 fraction and density are linearly correlated in amorphous carbon (a-C) and hydrogenated amorphous carbon (a-C:H) ®lms. Ó 2000 Elsevier Science B.V. All rights reserved. The properties of diamond-like carbons (DLCs) depend primarily on the fraction of sp3 and sp2 sites, the hydrogen content and the ordering of sp2 sites . At present electron energy loss spectroscopy (EELS) is the preferred method to determine sp3 fraction, because this method not only gives the sp2 content from the relative size of the p peak on the carbon K edge, but also the valence plasmon at 26±34 eV gives the mass density, which is often proportional to the sp3 fraction . However, EELS is a destructive and time-consuming method, so other non-destructive methods would be valuable. This paper describes advances in the use of two widely available, non-destructive methods, glancing angle X-ray re¯ectivity (XRR) * Corresponding author. Tel.: +44-1223 33 2689; fax: +441223 33 2662. E-mail address: [email protected] (J. Robertson). to give the ®lm density , and secondly Raman and ultraviolet (UV) Raman scattering to provide information on sp3 content. The refractive index of materials to X-rays is just under 1, so that X-rays are totally internally re¯ected within the air when incident at a grazing angle. The critical angle hc for total internal re¯ection is given by  1=2 NA r0 q XC ZC XH ZH ; 1 hc k p XC MC XH MH where k is the X-ray wavelength, r0 e2 =4p0 mc2 the classical electron radius, MC the molar mass of carbon, NA the Avogadro's number, Zi are the atomic numbers, Xi the atomic fractions, and q is the mass density. Writing XC 1 ÿ XH , the mass density q becomes q p2 c2 0 12 ÿ 11XH MC Me h2c : 2 2 6 ÿ 5XH 3k NA e 0022-3093/00/$ - see front matter Ó 2000 Elsevier Science B.V. All rights reserved. PII: S 0 0 2 2 - 3 0 9 3 ( 0 0 ) 0 0 0 3 5 - 1 2 766 A.C. Ferrari et al. / Journal of Non-Crystalline Solids 266±269 (2000) 765±768 Fig. 1 shows the re¯ected intensity from a tetrahedral amorphous carbon (ta-C) ®lm on a silicon substrate. The re¯ected intensity drops sharply above hc , and shows a series of oscillations as it declines. For high density carbon ®lms such as taC, the main critical angle is due to the C ®lm. However, lower density ®lms on Si such as a-C:H have an electron density less than Si, so the main hc is from the a-C:H/Si interface, and the a-C:H/air interface gives a subsiduary critical angle at a smaller angle. The intensity oscillations beyond hc due to the interference between beams re¯ected from the surface and substrate/®lm interface give the ®lm thickness. The longer period oscillation is due to internal layering. The complete information on density, ®lm thickness, surface roughness and the presence of internal layering is obtained by modelling the re¯ections from the ®lm/substrate pair. In this way, XRR can give the density and thickness of carbon ®lms to high precision (0.05 g/ cm3 and 0.1 nm) . The mass density was previously derived from valence plasmon energy, Ep , measured by EELS 1=2 using Ep h ne2 =e0 m or Fig. 1. X-ray re¯ectivity vs scattering angle, for ta-C, ta-C:H and a-C:H ®lms on Si substrates. q e0 MC m Ep2 2 12h NA e2 ! 12 ÿ 11XH ; 4 ÿ 3XH 3 where n is the valence electron density, m the electron eective mass, e0 the permittivity of free space and Ep is in eV. Comparing the derivation of density from XRR and plasmon energies, Eqs. (2) and (3), the X-ray critical angle is proportional to the total number of electrons, whereas the plasmon energy is proportional to the valence electrons. Thus, XRR density is less sensitive to H content than the plasmon energy, which is an advantage as H content is often less well known. Eq. (3) assumes that valence electrons behave like free electrons. This approximation works, but it is necessary to use an electron eective mass m of 0.85 to give the observed plasmon energy of diamond (33.8 eV). It is unclear if the same m holds for all carbons. Taking the mass densities of various carbon ®lms found by XRR and plasmon energies, we ®nd that m 0:87 gives a common ®t to all plasmon energies, so this approximation holds . Fig. 2 shows the density derived by XRR and from plasmon energies with this m value plotted against sp3 fraction for ta-C deposited by a ®ltered cathodic vacuum arc (FCVA) and ta-C:H deposited by plasma beam source (PBS) or by an electron cyclotron wave resonance (ECWR) system. Fig. 2. Variation of density with sp3 fraction for ta-C ®lms grown by FCVA and ta-C:H ®lms grown by PBS and ECWR. Lines are guide to eye. A.C. Ferrari et al. / Journal of Non-Crystalline Solids 266±269 (2000) 765±768 The density and sp3 content varies roughly linearly for the two types of DLCs. The highest density for ta-C is 3:26 0:05 g/cm3 for 88% sp3 fraction, whereas the ta-C:H has a lower density of 2.36 g/ cm3 for 70% sp3 fraction. The sp3 fraction is found from the carbon K edge EELS spectrum. The sp2 fraction is derived by taking the ratio of areas of the 285 eV peak due to p states and 290 eV edge due to r states, and comparing this to their ratio in graphite which is 100% sp2 . Raman scattering using visible photons is a popular method to probe the quality of CVD diamond and DLC. However, the visible Raman spectra of DLCs is dominated by the sp2 sites, which have a 55 times larger cross-section than sp3 sites, because visible photons are only able to excite p states. The Raman spectra of carbons is dominated by two features, a G peak at around 1550 cmÿ1 and a D mode around 1350 cmÿ1 . The G peak is derived from the zone centre E2g bond stretching mode of graphite, and is present in all sp2 bonded carbons. The D mode is a disorderactivated K zone boundary mode, due to the A1g symmetry breathing motion of 6-fold aromatic rings, which requires the presence of such rings. The interesting feature of Raman in disordered carbon is that the Raman spectra are dominated by these two features, rather than resembling the phonon density of states as it does in a-Si . A detailed analysis of the variation of the Raman spectra of carbon on their bonding ®nds that the spectra depend fundamentally on the ordering of the sp2 sites : whether sp2 sites form rings or chains, the density of aromatic rings, and the size of the aromatic ring clusters. If the sp3 and sp2 phases in DLCs are related, for example by the deposition process, so that the ordering of the sp2 phase evolves as the sp3 fraction increases, then we may use Raman spectra to derive sp3 content empirically. Fig. 3(a) shows the G peak wavenumber (measured at 514 nm) plotted against (Tauc) optical gap for plasma deposited a-C:H from data of Tamor and Vassell . We previously found that the optical gap of a-C:H varies systematically with sp3 content derived from EELS or NMR  (Fig. 4). This variation allows us to plot G wavenumber 767 Fig. 3. G peak wavenumber vs: (a) optical (Tauc) gap and (b) sp3 fraction, for as-deposited a-C:H ®lms (data from Tamor and Vassell ) for excitation at 514 nm. Fig. 4. Tauc gap vs sp2 content for various a-C and a-C:H ®lms . Lines are guide to eye. 768 A.C. Ferrari et al. / Journal of Non-Crystalline Solids 266±269 (2000) 765±768 Fig. 5. UV (244 nm) Raman spectra of ta-C, ta-C:H and a-C:H and a visible Raman spectrum of a-C:H. and ole®nic chains in diamond-like a-C:H, to shorter ole®nic chains in polymeric a-C:H, and this process causes the G peak to shift downwards. The sp3 sites are not directly observed in visible Raman. The higher photon energies of UV Raman can excite the r states of sp3 sites. The UV Raman spectra of ta-C shows a new broad peak at 1100 cmÿ1 labeled as T peak, attributed to sp3 sites  (Fig. 5) The G peak is still present in UV Raman, and has now moved to a higher wavenumber. It is found that the ratio of areas of T to G peak correlates well with the sp3 content for ta-C . The UV Raman spectra of other DLCs such as ta-C:H and a-C:H have been measured (Fig. 6). There is now a much broader feature below the G peak instead of a single T peak. There are a number of contributions to this feature, including C±H bending modes, which need to be further studied. Thus, the ratio of T to G peak areas is a rough guide to the sp3 content , but further work is needed to provide a reliable relationship. References Fig. 6. Variation of UV Raman T to G peak area vs sp3 fraction for various carbon ®lms. against sp3 content (Fig. 3(b)). It is seen that the G peak decreases almost linearly with increasing sp3 content, and may saturate at the highest sp3 content. As the sp3 content increases in a-C:H, the sp2 site ordering changes from aromatic clusters at large sp2 content, through single aromatic rings  J. Robertson, Prog. Solid State Chem. 21 (1991) 199.  P.J. Fallon, V.S. Veerasamy, C.A. Davis, J. Robertson, G.A.J. Amaratunga, W.I. Milne, J. Koskinen, Phys. Rev. B 48 (1993) 4777.  F. Toney, S. Brennan, J. Appl. Phys. 66 (1989) 1861.  A. Li Bassi, A.C. Ferrari, V. Stolojan, B.K. Tanner, J. Robertson, L.M. Brown, Diamond Related Mater. (2000) in press.  R.J. Nemanich, S.A. Solin, Phys. Rev. B 20 (1979) 392.  R. Alben, D. Weaire, J.E. Smith, M.H. Brodsky, Phys. Rev. B 11 (1975) 2271.  A.C. Ferrari, J. Robertson, Mater. Res. Soc. Symp. Proc. 593 (1999).  M.A. Tamor, W.C. Vassell, J. Appl. Phys. 76 (1994) 3823.  J. Robertson, Phys. Rev. B 53 (1996) 16302.  K.W.R. Gilkes, H.S. Sands, D.N. Batchelder, J. Robertson, W.I. Milne, Appl. Phys. Lett. 70 (1997) 1980.  S. Prawer, K.W. Nugent, in: S.R.P. Silva et al. (Eds.), Amorphous Carbon State of Art, World Scienti®c, Singapore, 1998.  G. Adamopoulos, K.W.R. Gilkes, J. Robertson, N.M.J. Conway, B.Y. Kleinsorge, A. Buckley, D.N. Batchelder, Diamond Related Mater. 8 (1999) 541.